Survey

* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project

Document related concepts

Electrical resistivity and conductivity wikipedia, lookup

Lorentz force wikipedia, lookup

Centripetal force wikipedia, lookup

Aharonov–Bohm effect wikipedia, lookup

Electromagnet wikipedia, lookup

Electrical resistance and conductance wikipedia, lookup

Superconductivity wikipedia, lookup

Electromagnetism wikipedia, lookup

Work (physics) wikipedia, lookup

Time in physics wikipedia, lookup

Classical central-force problem wikipedia, lookup

History of fluid mechanics wikipedia, lookup

Newton's laws of motion wikipedia, lookup

Equations of motion wikipedia, lookup

High-temperature superconductivity wikipedia, lookup

Potential energy wikipedia, lookup

Transcript

INFLUENCE OF THE AC CURRENT ON THE NONLINEAR DC RESISTIVE RESPONSE IN A TILTED WASHBOARD PINNING POTENTIAL Oleksandr V. Dobrovolskiy1,2 1 2 Kharkov National University, Physical Department, 61077 Kharkov, Ukraine Physikalisches Institut, Goethe-Universität, 60438 Frankfurt am Main, Germany ABSTRACT Influence of the ac current on the longitudinal and transverse (with respect to the dc current direction) even and odd (with respect to the magnetic field reversal) – dependent nonlinear anisotropic magnetoresistivities , of a type-II superconductor is considered. The current and frequency dependence of the number and position of the Shapiro-like steps on the current-voltage characteristic is calculated and analyzed for the transverse geometry at low temperatures. A simple physical picture of the vortex motion in a washboard periodic pinning potential, tilted due to the presence of the dimensionless dc driving force, is elucidated. INTRODUCTION It is well known that the mixed-state resistive properties of type-II superconductors are determined by the dynamics of vortices which again are strongly influenced by distribution of pinning sites [1]. In the simplest case this distribution is assumed to be periodic in one dimension, and temperature-dependent dc current uniaxial pinning anisotropy, provoked by such washboard planar pinning potential (PPP) recently has been extensively studied both theoretically [2-4] and experimentally [5-9]. As the pinning force in a PPP is directed perpendicular to the washboard channels of the PPP [1], the vortices generally tend to move along these channels. Such a guided motion of vortices in the presence of the Hall effect produces anisotropic transport behaviour for which even (+) and odd (–) with respect to the magnetic field reversal, longitudinal ( ) and transverse ( ) dc nonlinear magnetoresistivities , depend substantially on the angle α between the dc current density vector j and the direction of the PPP channels ("guiding direction"). The dc-current nonlinear guiding problem was exactly solved recently for the washboard PPP within the framework of the two-dimensional (2D) single-vortex stochastic model of anisotropic pinning based on the Fokker-Planck equation and rather simple formulas were derived for the dc magnetoresistivities , [2,3]. Thereupon the (dc+ac)-current nonlinear guiding problem was exactly solved in the frames of the Langevin equation [10] in terms of a matrix continued fraction [11] without the recourse to the Fokker-Planck approach. As a result, two groups of new findings were obtained in Ref. [10]. First, for the previously solved in Refs. [2, 3] 2D dc–problem the influence of an ac current on the anisotropic dc, dc-response was calculated and analyzed. Second, for the ac current at a frequency plus dc bias the 2D nonlinear time-dependent stationary ac, 1-245 ac-response on the frequency in terms of nonlinear impedance tensor Z and a nonlinear ac response at -harmonics were studied. In the present paper we discuss the influence of the ac current on the overall shape and appearance of the Shapiro-like steps on the dc current-voltage characteristics (CVC) pointed out in Ref. [10] and propose a simple physical picture of the vortex motion in a washboard periodic pinning potential, tilted due to the presence of the dimensionless dc driving force. MAIN RESULTS The Langevin equation for a vortex moving with velocity v in a magnetic field B = nB (B ≡ |B|, n = nz, z is the unit vector in the z-direction and n = ±1) has the form ηv + nαH v x z = FL + Fp + Fth , (1) where FL = n(Ф0./c) j x z is the Lorentz force, Ф0 is the magnetic flux quantum, c is the speed of light, j = j(t) = jdc + jac cos ωt, where jdc and jac are the dc and ac current density amplitudes and ω is the angular frequency, Fth is the thermal fluctuation force represented by a Gaussian white noise with zero mean [2,3], η is the vortex viscosity, αH is the Hall constant, Fp = - Up(x) is the anisotropic pinning force and we assume, as usual [2,10] an a-periodic pinning potential of the form Up(x) = (Up/2)(1-coskx) where k = 2π/a. The main quantity of physical interest in our problem is the average electric field, induced by the moving vortex system, which is given by E (n / c)B v n( B / c)( v y x vx y ), (2) where x and y are the unit vectors in the x and y directions, respectively. As follows from Eq. (1) v y FLy / vx where n , H / , and so for determination of E from Eq. (2) it is sufficient to calculate the vx from Eq. (1). This calculation gives vx (t ) (Ф0 jc / c D)[ j dc j ac cos t sin x (t )], (3) where D 1 2 , j dc n( j ydc jxdc ) / jc , j ac n( j yac jxac ) / jc , with jc cFp / Ф0 , j y j cos , jx j sin , sin x (t ) (i / 2)[ r (t ) r 1 (t )], r (t ) exp[ ix(t )], and x kx. Looking for only the stationary ac response, which is independent of the initial condition, one may seek all the r m (t ) in the form [11] r m (t ) F k m k ( )eikt . (4) On substituting Eq. (4) into Eq. (3) we obtain recurrence equations for the (jac, jdc, Ω, g)-dependent Fourier amplitudes Fkm , where g = (Up/2T), T is the temperature in energy units, is the dimensionless frequency and D / kFp 1-246 is the relaxation time. From the solution of these recurrence equations in terms of matrix continued fraction, as detailed in Refs. [10, 11], we can find the dimensionless average pinning force Fpx (t ) which is the main anisotropic nonlinear, due to αdependence on the ac and dc current input, component of our theory F px (t ) sin x (t ) Im( k eikt ) (5) k 0 where 0 F01 ( ) and for k 1 we have k Fk1 ( ) Fk1 ( ) . From Eq. (5) we can decompose average pinning force F px (t ) into three components F px (t ) F px F px 0 In Eq. (6) sin x F px 0 k 1 F px t1 (6) . t Im 0 is the time independent (but frequency 0 sin x dependent) static average pinning force; F px t1 Im( 1eit ) is the time- t1 dependent dynamic average pinning force with a frequency ω of the ac current input; k 1 sin x F px k 1 Im( k eikt ) t describes a contribution of the harmonics with t k > 1 into the dynamic average pinning force. In order to derive the ω-dependent nonlinear dc resistivity and conductivity tensors we first express (see Eq. (2)) the time independent part of E y (t ) and Ex (t ) as Ey Ex 0 0 ( f / D) 0 ( j ydc jxdc ), (7) ( f / D)[ j (1 (1 0 )) j ]. dc x 2 Here ρf ≡ BФ0/ηc is the flux-flow resistivity, 0 1 sin x 2 dc y 0 / j 1 F px dc / j dc 0 0 where at j = 0 can be considered as the probability of vortex hopping over the pinning potential barrier under the influence of the dimensionless generalized moving ac force FLxdc j dc in the x direction [3]. From Eqs. (7) we find the magnetoresistivity tensor for the dc nonlinear law E0 ( ) 0 jdc as xxdc xydc f D 2 0 0 dc dc D yx yy 0 0 . 0 (8) The dc conductivity tensor 0 , which is the inverse tensor to 0 , has the form xxdc xydc 1 1 0 dc dc . 2 f ( D / 0 ) yx yy (9) We see from Eqs. (8) and (9) that the off-diagonal components of the 0 and 0 tensors satisfy the Onsager relation (ρxy = – ρyx in the general nonlinear case and σxy = – σyx). 1-247 The experimentally observable longitudinal and transverse (with respect to the j direction) dc magnetoresistivities dc E dc / j and dc Edc / j (where jd is the dc current density ( j d )2 ( jxdc )2 ( j ydc )2 have the form dc ( f / D)[( D 2 0 )sin 2 0 cos 2 ], (10) dc ( f / D)[ 0 D(1 0 )sin cos ], where in order to separate the even and odd components of dc, we should use 0 (n) [ 0 (n) 0 (n)] / 2 which are the even and odd components (relative to the magnetic field inversion) of the function 0 (n) (compare with Eqs. (13)-(14) in Ref. [4]). DISCUSSION Below we present a graphical analysis of Ω-dependent dc nonlinear response calculated in the transverse (α = 0) T-geometry (the current density vector is parallel to the pinning channels, see details in Ref. [3]) at low temperatures (g > 10). However, it is instructive to consider first a simple physical picture, shown in Fig. 1, of the vortex motion in a washboard planar pinning potential (PPP), tilted due a presence of the dimensionless dc driving force 0 < ξd < ∞, under the influence of the effective dimensionless driving force f Fpx FLx sin x d . Hear and further ξd ≡ jd/jc and ξa ≡ ja/jc are the dimensionless dc and maximal ac current density magnitudes in jc units, respectively. If the temperature is zero, the vortex is at rest with ξd = 0 at the bottom of the potential well of the PPP. When the PPP is gradually lowered by increasing ξd, then for 0 < ξd < 1 appears an asymmetry of the left-side and right-side potential barriers for a given potential well, and in this range of ξd an effective force f changes its sign periodically. With gradual ξd -increasing there will come a point where ξd = 1, and for ξd > 1 the more lower right-side potential barrier disappears, the effective motive force f becomes everywhere along x positive and the vortex is in the "running" state, periodically changing its velocity with a dimensionless frequency i ( d ) 2 1 . So the static CVC of this periodic motion at ξd > 1 is a result of time-averaging of the stationary time-dependent solution of the equation of motion dx/dτ = f with t / . Eventually, the probability of the vortex overcoming the barriers of the PPP 0 0 ( a 0, 0) at zero temperature is 0, 0 d 2 1 (1/ ) d 1, d 1, i. e. 0 ( d 1) monotonically tends to unity with ξd-increasing. 1-248 (11) If the temperature is nonzero, a diffusion-like mode appears in the vortex motion. At low temperatures ( g 1 ) and 0 < ξd < 1 the thermoactivated flux-flow Fig. 1. Modification of the effective pinning potential U(x) ≡ Up(x) – Fx with gradual increasing of the Lorentz force F F Lx , where Up(x) – is a periodic pinning poten tial. If the condition F Fp F px is satisfied, the initial potential well (with its depth U0 and width a) is tilted with a storing of the average vortex position. When F = Fp, the right-side potential barrier disappears. At last, when F > Fp, the vortex motion direction coincides with a direction of the moving force F. (TAFF) regime of the vortex motion occurs by means of the vortex hopping between neighboring potential wells of the PPP. The intensity of these hops at low temperatures is proportional to the exp[ g (1 d )] , i. e. strongly increases with Tincreasing and ξd-increasing due to the lowering of the right-side potential barriers at their tilting. On the other hand, at ξd just above the unity (when the running mode is yet weak), the diffusion-like mode can strongly increase the average vortex velocity even at relatively low temperature due to a strong enhancement of the effective diffusion coefficient of an overdamped Brownian particle in a tilted PPP near the critical tilt [12] at ξd = 1. Now we consider the influence of a small ( a 1 ) ac current density with a frequency ω on the CVC in the limit of very small temperatures ( g 1 ). In this case the physics of the dc response is quite different depending on the ξd value with respect to the unity. If ξd < 1, the vortex mainly (excluding very rare hops to the neighboring wells) localized at the bottom of the potential well where it experiences small ωoscillations. The averaging of the vortex motion over the period of oscillations in this case cannot change the CVC which existed in the absence of the ac-drive. If, however, ξd > 1, then the vortex is in running state with the internal frequency of oscillations i ( d ) 2 1 . If i , the CVC is changed only in the second-order perturbation approach in terms of a small parameter a 1-249 1 (as it was shown for the analogous resistively shunted Josephson junction problem [13]) because the CVC is not changed in the linear approximation in this case. However, Fig. 2. The longitudinal CVC E dc,T ( d ) for Ω = 0.05(1), 0.1(2), 0.2(3), 0.3(4), 0.5(5) with ξa = 1 and g = 50. Dotted lines correspond to the Ohm`s law E dc,T = ξd. The curves 2 – 5 are shifted by 1 along the ξd-axis for clarity. for i appears a problem of a synchronization of the running vortex oscillations at the ωi-frequency with the external driving frequency ω. As a result, the average over period of oscillations vortex velocity is locked in with the ω in some interval of the dc current density ξd even within the frame of the first-order perturbation calculation (see Fig. 2). The width of this first synchronization step (or the so-called "Shapiro step" in the resistively shunted Josephson junction problem) has been found in Ref. [14] and the calculation in the spirit of this reference gives the boundaries of the ξd where the step occurs as (d a / 2 d ) d (d a / 2 d ). (12) Here ξd is the current density which gives i (d )2 1 , i. e. d 1 2 . Then the size of the first Shapiro-like step on the CVC is a / d . In higher approximations (in terms of (ξa)n), where n runs through all of the integers) the Shapiro-like steps on the CVC appear at the frequencies n and i ni . The width of the n-th step at a 0 is proportional to (ξa)n, i. e. strongly decreases with n increasing [15]. In Fig. 3 we plot the longitudinal CVC E dc,T ( d ) for various ξa showing the “Shapiro” steps. The plot in Fig. 3 looks like the similar curves discussed earlier [16] for the CVC of the microwave driven resistively shunted Josephson junction model at T = 0 where the overall shape of the CVC and different behaviour of the two types of the Shapiro steps in adiabatic limit was explained. Our graph, in comparison with the curves of Ref. [16], is smoothed due to the influence of a finite temperature. The longitudinal CVC E dc,T ( d ) -dependence demonstrate several main features. First, in 1-250 the presence of the microwave current the dc critical current cd ( a ) is a decreasing function of the ac driving. The physical reason for such behaviour lies in the replacement of the dc critical current by the total dc + ac critical current. Second, Fig. 3. The longitudinal CVC E dc,T ( d ) is calculated for ξa =0.01(1), 0.5(2), 1(3), 1.5(4), 2(5) with Ω = 0.2, and g = 50. Dotted lines correspond to the Ohm`s law E dc,T d . The curves 2 – 5 are shifted by 1 along the ξd-axis for clarity. with gradual ξa-increasing the zero-voltage step reduces to zero and all other steps appear. Such steps are common because they do not oscillate and spread over a dccurrent range about twice the critical current 2 ca . These steps are the steps of the first kind and they distort the CVC as like as relief bump with a concave shift from the ohmic line. With further ξa-increasing this relief bump shifts toward higher ξdvalues. Below this range the steps of the second kind appear. These microwave current-induced steps oscillate rapidly and stay closely along the ohmic line over a dccurrent range d a 1 . To summarize, we can determine three (ξd, ξa)-ranges where the CVC-behaviour is qualitatively different. In particular, for large dc bias current densities ξa+1 < ξd the CVC asymptotically approaches the ohmic line without microwave induced steps. For an intermediate dc current range occurs as ξa – 1 < ξd < ξa + 1 CVC curve deviates from the ohmic line as a concave bump with the stable steps. For lower dc current range ξd < ξa – 1 the steps oscillate with microwave current along the ohmic line. With gradual Ω-increasing the size of the steps increases whereas their number decreases. CONCLUSION In the present work we have theoretically examined the influence of the ac current on the anisotropic dc current-voltage characteristic of a type-II superconductor in the mixed state. A simple physical picture of the vortex motion in a tilted washboard periodic pinning potential has been proposed and elucidates a rich physics arised from the combination of a dc and ac driving, and the low temperature mediated vortex hopping (or running) in a washboard pinning potential. Experimental realization of this model in thin-film geometry [8, 9, 17] opens up the possibility for a variety of 1-251 experimental studies of directed motion of vortices under (dc+ac) – driving simply by measuring longitudinal and transverse voltages. Experimental control of a frequency and value of the driving forces, damping, Hall constant, pinning parameters and temperature can be effectively provided. ACKNOWLEDGEMENTS The work was supported in part by the DAAD fellowship grant No. A/08/96378. The author deeply appreciates the useful discussions with Valerij A. Shklovskij and gratefully acknowledges Michael Huth for the financial support in the frames of the NanoBic research project. REFERENCES [1] Blatter G., Feigel'man M. V., and Geshkenbein V. B: 'Vortices in high-temperature superconductors'. Rev. Mod. Phys. 1994 66 (4) 1125-1388. [2] Mawatari Y: 'Dynamics of vortices in planar pinning centers and anisotropy conductivity in type-II superconductors'. Phys. Rev. B 1997 56 (6) 3433-3437; Anisotropic current-voltage characteristics in type-II superconductors with planar pinning centers'. Phys. Rev. B 1999 59 (18) 12033-12038. [3] Shklovskij V. A., Soroka A. A., and Soroka A. K: 'Nonlinear dynamics of vortices pinned to unidirectional twins'. J. Exp. Theor. Phys. 1999 89 (6), 1138-1153. [4] Shklovskij V. A. and Dobrovolskiy O. V: 'Influence of point-like disorder on the guiding of vortices and the Hall effect in a washboard planar pinning potential'. Phys. Rev. B 2006 74 104511-1–14. [5] Chabanenko V. V., Prodan A. A., and Shklovskij V. A: 'Guiding of vortices in YBa2Cu3O7±δ single crystals with unidirected twins'. Physica C 1999 314 133-138. [6] Pastoriza H., Candia S., and Nieva G: 'Role of twin boundaries on the vortex dynamics in YBa2Cu3O7±δ '. Phys. Rev. Lett. 1999 83 (5) 1026-1029. [7] D'Anna G. et. al: 'Scaling of the Hall resistivity in the solid and liquid vortex phases in twinned single-crystal YBa2Cu3O7±δ '. Phys. Rev. B. 2000 61 (6) 4215-4220. [8] Huth M., Ritley K. A., and Oster J: 'Highly ordered Fe and Nb stripe arrays on facetted α-La2O3(1010)'. Adv. Funct. Mater. 2002 12 (5) 333-338. [9] Soroka O. K., Huth M., and Shklovskij V. A: 'Guiding of vortices under competing isotropic and anisotropic pinning conditions'. Phys. Rev. B 2007 76 014504–1-12. [10] Shklovskij V. A. and Dobrovolskiy O. V: 'AC-driven guiding of vortices and the Hall effect in a tilted washboard planar pinning potential'. Phys. Rev. B. 2008 78 104526–1-15. [11] Coffey W. T., Dejardin J. L., and Kalmykov Yu. P: 'Nonlinear impedance of a microwave-driven Josephson junction with noise'. Phys. Rev. B 2000 62 (5), 3480-87. [12] Riemann P., Van den Broeck C., and Linke H.: 'Giant acceleration of free diffusion by use of tilted periodic potential'. Phys. Rev. Lett. 2001 87 010602-06. [13] Kanter H. and Vernon F. L: 'High-frequency response of Josephson point contacts'. J. Appl. Phys. 1972 43 3174-83. [14] Aslamazov L. G. and Larkin A. I: 'Josephson effect in point superconducting contacts'. JETP Lett. 1969 9 (2) 150-54. [15] Likharev K. K. and Ulrich B. T: Systems with Josephson Contacts. Moscow, MSU, 1978. 1-252 [16] Vanneste C. et al: 'I-V characteristics of microwave-driven Josephson junctions in the low-frequency and high-damping regime'. Phys. Rev. B 1985 31 (7) 4230-33. [17] Dobrovolskiy O. V., Huth M., and Shklovskij V. A: 'Fabrication of Artificial Anisotropic Pinning Structures in Thin Niobium Films Sputtered onto Sapphire Substrates'. Int. Conf. on Supercond. and Magnetism, Antalya, Turkey, 2010. 1-253